sensitization of the lanthanides, and that has been revealed by
its photophysical properties.
■ EXPERIMENTAL SECTION
Materials and General Procedure. All the reagents and solvents
were commercially available and were used as obtained. Pamoic acid,
Gd(NO3)3·6H2O, and Dy(NO3)3·6H2O were obtained from the
Sigma Aldrich Chemical Company and used as received.
The elemental analyses were carried out on Elementar Micro vario
Cube elemental analyzer. FT-IR spectra (4000−400 cm−1
recorded on KBr pellets with a Perkin-Elmer Spectrum BX
spectrometer. Cary Eclipse EL05033882 was used for ﬂuorescence
spectra. Powder X-ray diﬀraction (PXRD) data were collected on a
PANalytical EMPYREAN instrument, using Cu Kα radiation. In order
to evaluate the porous property of both complexes, the crystalline
materials are grounded to powder and activated by drying under
vacuum at 100 °C for 10 h. Gas and solvent vapor adsorption studies
were performed using a BELSORP MAX (BEL JAPAN) volumetric
adsorption analyzer. Magnetic measurements were performed using a
Quantum Design SQUID VSM magnetometer. The measured values
were corrected for the experimentally measured contribution of the
sample holder, while the derived susceptibilities were corrected for the
diamagnetism of the samples, estimated from Pascal’s tables.19
Crystal Data Collection and Structure Determination.
Suitable single crystals of each of the complexes were mounted on a
Bruker SMART diﬀractometer equipped with a graphite mono-
chromator and Mo Kα (λ = 0.71073 Å, 140 K) radiation. Data
collection was performed using ϕ and ω scans. The structures were
solved using direct methods followed by full matrix least-squares
reﬁnements against F2
(all data HKLF 4 format) using SHELXTL.20
Subsequent diﬀerence Fourier synthesis and least-squares reﬁnement
revealed the positions of the remaining nonhydrogen atoms.
Determinations of the crystal system, orientation matrix, and cell
dimensions were performed according to the established procedures.
Lorentz polarization and multiscan absorption correction were applied.
Nonhydrogen atoms were reﬁned with independent anisotropic
displacement parameters, and hydrogen atoms were placed geometri-
cally and reﬁned using the riding model. All calculations were carried
out using SHELXL 97,21
and WinGX system, version
The solvent DMF molecules in 1 and 2 are highly disordered,
and attempts to locate H atoms on the calculated positions by riding
method (for 1) were unsuccessful, which results in a larger Hirschﬁeld
diﬀerence for N1−C38 and C36. Similarly, in 2, the DMF (C36, C38,
and N1) molecules are disorderd. Since both the complexes show
solvent accessible voids, SQUEEZE23
was used, and a new .HKL ﬁle
was generated. The structure was solved by using the newly generated
.HKL ﬁle. Structure reﬁnement after modiﬁcation of the data with the
SQUEEZE routine led to better reﬁnement and data convergence.
Detailed instruction from the .SQF ﬁle is included in the ﬁnal .cif ﬁle.
From the TG analysis, it is conﬁrmed that only one noncoordinated
DMF molecule are present, which is removed by the SQUEEZE
program and, hence, included in the molecular formula. Data
collection and structure reﬁnement parameters and crystallographic
data for the two complexes are given in Table 1.
Synthesis of [Gd2(pam)3(DMF)2(H2O)2]n·nDMF (1). To a 10 mL
solution of methanol and DMF (1:1), Gd(NO3)3·6H2O (0.2 mmol, 90
mg) was added, and the solution was stirred for 10 min to dissolve
completely. To this solution, pamoic acid (0.3 mmol, 116.5 mg) was
added part-by-part, and stirring of the solution continued. After 15
min, 2 drops of pyridine were added and allowed to stir for 1 h more.
The solution was then ﬁltered, and the ﬁltrate was kept for
crystallization at room temperature. After one day, pale yellow single
crystals were separated by ﬁltration, washed with DMF, and dried in
air. Yield: 170 mg (52%). Elemental analysis (%): Calcd (found) for
C78H67Gd2N3O23: C, 54.19(53.84); H, 3.91(3.45); N, 2.43(2.13).
Selected IR data (4000−400 cm−1
, KBr pellet): 3412(b), 1648(s),
1546(m), 1399(s), 1349(m), 1329(w), 1303(w), 1029(s), 912(w),
812(s), 749(s), 601(s), 437(w).
Synthesis of [Dy2(pam)3(DMF)2(H2O)2]n·nDMF (2). Complex 2
was prepared following the same procedure used for 1, using
Dy(NO3)3·6H2O (0.2 mmol, 91 mg) instead of Gd(NO3)3·6H2O.
After one day, pale yellow single crystals were separated by ﬁltration,
washed with DMF, and dried in air. Yield: 162 mg (49%). Elemental
analysis (%): Calcd (found) for C78H67Dy2N3O23: C, 53.86(53.32); H,
3.88(3.57); N, 2.42(2.16). Selected IR data (4000−400 cm−1
pellet): 3415(b), 1642(s), 1383(s), 1346(m), 1327(w), 1300(w),
1237(s), 1204(s), 1153(w), 1094(s), 957(m), 880(m), 758(s),
680(w), 601(s), 439(w).
■ RESULTS AND DISCUSSIONS
We used pamoic acid as building blocks for several reasons: (1)
it exhibits a long distance between two coordination points of
the carboxylate group, which makes it convenient to act as a
spacer in building a porous network; (2) it possesses both
rigidity from the naphthyl rings and ﬂexibility from the twisted
C−CH2−C single bond, which could lead to a possible helical
architecture; (3) it exhibits delicate π−π stacking interactions,
which often plays a decisive role in regulating supramolecular
networks; and (4) its metal complexes can be used as electrical
conductors as well as potential ﬂuorescent materials.24
synthesis of 1 and 2, few drops of pyridine have been added to
facilitate deprotonation of pamoic acid. Although triethylamine
does the same job, the crystals isolated using pyridine are of
better diﬀracting qualities than that of triethylamine. The
absence of characteristic absorption of νas(COOH) near 1700
indicates that pamoic acid is completely deprotoned in
both complexes. The νas(COO−
) vibration of the carboxylate
group occurs at 1648 and 1642 cm−1
for 1 and 2, respectively,
while those of νs(COO−
) occur at 1399 and 1383 cm−1
respectively. The large diﬀerence in the Δ(νas−νs) values of
for 1 and 243−310 cm−1
for 2 evidence the
presence of both chelating bidentate and bis-monodentate
Table 1. Summary of X-ray Crystallographic Data for 1 and
CCDC number 941734 942172
formula C78H67Gd2N3O23 C78H67Dy2N3O23
formula mass 1728.87 1739.37
wavelength (Å) 0.71073 0.71073
temperature (K) 140 140
crystal system monoclinic monoclinic
space group C2/c C2/c
a (Å) 31.517(12) 31.28(3)
b (Å) 14.882(4) 14.735(13)
c (Å) 28.494(8) 28.51(5)
α (deg) 90.00 90.00
β (deg) 120.19(2) 120.13(5)
γ (deg) 90.00 90.00
) 11552(6) 11365(24)
Z 4 4
D ( C/g−3
) 0.942 0.972
μ (Mo Kα) (cm−1
) 1.186 1.353
F(000) 3240 3312
reﬂection 13267 13215
unique 13041 9604
GOOF on F2
[I > 2σI] 0.0623 0.0737
[I > 2σI] 0.1532 0.1251
(Δρ)max, (Δρ)min (e A−3
) 1.023, −1.007 1.131, −1.321
R1 = Σ∥Fo| − |Fc∥/Σ|Fo| and wR2 = |Σw(|Fo|2
Crystal Growth & Design Article
dx.doi.org/10.1021/cg401804e | Cryst. Growth Des. 2014, 14, 1287−12951288
mode of pamoates (Scheme S1 of the Supporting Informa-
TG analysis (Figure S1 of the Supporting Information)
shows a weight loss of ∼5% (calculated ∼4%) in the
temperature range of 120−160 °C, which might be due to
the loss of one noncoordinated DMF molecule from the
framework. The desolvated framework displays a weight loss of
∼10% (calculated ∼10%) in the temperature range of 180−290
°C, which corresponds to the loss of two coordinated water and
two DMF molecules from the frameworks. The bulk phase
powder X-ray diﬀraction patterns of both complexes is in good
agreement with the simulated one based on the single crystal
structure data (Figure S2 of the Supporting Information),
indicating the purity of the as-synthesized product.
Structural Description for Complexes 1(Gd) and
2(Dy). Single-crystal X-ray diﬀraction analysis reveals that
complexes 1 and 2 are isostructural in nature and crystallize in
the monoclinic space group C2/c. As illustrated in Figure S3(a)
of the Supporting Information, the asymmetric unit contains
similar core structure [Ln(pam)1.5(DMF)(H2O)] [where Ln =
Gd(1) and Dy(2)] having one Ln ion, one and half of pamoate
ligands, one DMF, and one coordinated water molecule. In
both complexes, each Ln centers are eight-coordinated with six
oxygen atoms from two pamoate ligands, one oxygen atom
from the DMF molecule, and one coordinated water molecule.
Thus the coordination arrangement around the Ln centers can
be described as a distorted square antiprismatic (Figure S3(b)
of the Supporting Information). The Ln−O bond lengths are in
the range of 2.297(4)− 2.458(5) Å for 1 and of 2.306(6)−
2.48(1) Å for 2, respectively. The relevant bond parameters
around the Ln centers are listed in Table S1 of the Supporting
Information. In both complexes, the ﬂexible skeleton of pam2−
is twisted, and the hydroxy and carboxyl groups adopt an anti
(staggered) conformation to minimize the steric hindrance. In
addition, intramolecular H-bonding interactions between them
further stabilize the conformation. The H-bond parameters are
listed in Table S2 of the Supporting Information. The dihedral
angles between two naphthyl moieties of two pamoate ligands
in 1 and 2 are diﬀerent and were found to be 77.77° and 82.44°
and 77.19° and 79.73°, respectively.
It is important to note that in both complexes, two pamoate
ligands uniquely adopt two diﬀerent bridging modes (Figure 1
and Scheme S1 of the Supporting Information) [i.e., one is in
both the monodentate and the chelating bidentate mode (type
I, left) and the other is in only the monodentate bridging mode
(type II, right) and can be viewed as μ3- and μ4-connectors,
respectively, to form a 2D framework having a channel of size
17.427 × 15.163 Å (for 1) and 14.58 × 17.23 Å (for 2), as
shown in Figure S4 of the Supporting Information]. Although
the channel size has been calculated taking Ln···Ln and CH2···
CH2 separations into consideration, the real volume of the
cavities are further reduced due to the signiﬁcant oﬀset stacking
of naphthyl moieties of pamoate inside the framework. The two
types of pamoates are arranged alternatively in the framework
(Figure S5 of the Supporting Information), where the
lanthanides are arranged like “tiles” on the ﬂoor (Figures S6
and S7 of the Supporting Information).
In overall, it can be seen that the noted extended two-
dimensional (2D) framework is formed by squashed metal-
lomacrocycles (Figure 2), originating from the basic secondary
building units (SBU) [Ln2(pam)6(DMF)2(H2O)2], as shown in
Figure S8 of the Supporting Information. Also, each SBU is
connected to six nearby SBUs through pamoate ligands.
Overall, its representation is similar to a dumble [Figure 3
(left)], and its schematic representation is illustrated in Figure 3
In the SBU, two types of pamoate ligands are coordinated to
lanthanide dimers (i.e., two type I and four type II). The Ln···
Ln distances in the unit are 4.229(1) Å for 1 and 4.214(3) Å for
2, respectively. The oxygen atoms of type II pamoates bridge
the lanthanide centers symmetrically, which results in a very
rare lanthanide paddle wheel structure [Figure S9(a) of the
Figure 1. Illustration of two types of bridging mode of pamoic acid
type I (left) and type II (right) observed in complexes 1 and 2.
Figure 2. Illustration of lanthanide metallomacrocycle found in 1.
Figure 3. Views representing the connection of each SBU to six nearby
SBUs though pamoate ligands, overall showing a dumble shape (left)
and its schematic view (right).
Crystal Growth & Design Article
dx.doi.org/10.1021/cg401804e | Cryst. Growth Des. 2014, 14, 1287−12951289
where pamoates form a dihedral
angle of 86.99°(1) and 88.97°(2), respectively. Each lanthanide
paddle wheel connected to six nearby units through the six
pamoate groups and extended in one-dimensional (1D)
fashion, as shown in Figure S9(b) of the Supporting
Information. For both complexes, the Ln···Ln separations
between the paddle wheels (between the SBUs) are ∼15 Å.
Viewing the lattice of 1 along the c axis illustrates helical
arrangement of lanthanide pamoates [right (P) and left-handed
(M)], which further extended to a 2D array by another V-
shaped pamoate, as shown in Figure 4. The helix generated
around the 21 screw axis exhibit a pitch of 14.88 Å (for 1) and
14.70 Å (for 2), respectively. Here it is very important to note
that in the framework, the usual π···π interactions between
naphthyl moieties are aﬀected by the intervening of another
naphthyl moiety in between them. Moreover, in the 3D
framework (Figure S10 of the Supporting Information), the
SBUs are organized through diﬀerent noncovalent interactions,
such as edge-to-face C−H···π and C−H···O interactions and
the naphthyl moieties are slipped over one another, having a
cg···cg distance of 5.316 Å. PLATON analysis26
pore-accessible volume of 53.9%, with respect to the whole unit
cell volume (6226.5 Å3
out of the 11552.0 Å3
per unit cell
volume) for complex 1 and 50.7% with respect to the whole
unit cell volume (5766.2 Å3
out of the 11365.0 Å3
per unit cell
volume) for complex 2, respectively.
Magnetic Property Studies. The bulk purity of both
complexes 1 and 2 were conﬁrmed by comparing the
corresponding simulated and experimental PXRD patterns
(Figure S2 of the Supporting Information). The DC magnetic
susceptibility data for 1 and 2 were collected in the temperature
range of 1.8−300 K at 1KG (Figures 5 and 6). The room
temperature χMT (χM = molar magnetic susceptibility) value
was found to be 15.36 cm3
K for 1 (calculated χMT =
K for two noninteracting Gd3+
S7/2, g =
1.99). The small diﬀerence between the calculated and
experimental χMT value is due to the antiferromagnetic
coupling between the Gd3+
centers. Upon cooling, this value
remains almost constant up to 30 K and decreases down to
reach a value of 14.11 cm3
K at 1.9 K. The shape of the
plot indicates the presence of weak antiferromagnetic
interactions between the Gd3+
centers. With consideration of
the dimeric core found in 1 (Figure S9(a) of the Supporting
Information), it can be assumed that the magnetic coupling was
occurring between two nearby Gd3+
ions through the bidentate
carboxylate bridging group. The above observed antiferromag-
netic coupling in complex 1 might be because of Ln···Ln
separation in the dimeric unit [Gd3+
, 4.229(1) Å] and
the chelating bidentate bridging mode of the carboxylate group
in the dimeric unit.28e
For complex 2, the obtained room
temperature χMT (χM = molar magnetic susceptibility) value is
K [Calculated χMT = 28.33 cm3
two uncoupled Dy3+
H15/2, g = 1.33)].
The molar magnetic susceptibility data of 1 and 2 were ﬁtted
according to the Curie−Weiss equation, χM = C/(T − θ),
which aﬀorded the Curie constants (C) = 15.35 cm3
for 1 and 27.63 cm3
K for 2 and Weiss constants (θ) =
−0.064 K for 1 and −3.97 K for 2 (Figure S11, panels a and b,
of the Supporting Information). For complex 1, negative value
of θ further conﬁrms the presence of antiferromagnetic (AF)
interaction between Gd3+
centers. But for complex 2, small
negative θ values do not imply the existence of antiferromag-
netic interaction between Dy3+
centers due to the presence of
large orbital angular momentum and strong spin−orbit
Figure 4. Illustration of helical chain [right (P) and left-handed (M)]
found in complex 1.
Figure 5. Temperature dependence of the DC susceptibility for
complex 1 (Gd) (inset magnetization curve).
Figure 6. Temperature dependence of the DC susceptibility for
complex 2 (Dy) (inset magnetization curve).
Crystal Growth & Design Article
dx.doi.org/10.1021/cg401804e | Cryst. Growth Des. 2014, 14, 1287−12951290
coupling for Dy3+
. In case of complex 2, the χMT value slowly
decreases down to 70 K and then decreases rapidly to a value of
K at 1.8 K, which is probably due to the
thermal depopulation of excited Stark sublevels in
Magnetization data for complex 1 was measured
in the temperature range from 2 to 10 K [Figure 5 (inset)],
which shows a steady increase with increasing ﬁeld (H) and
saturation values of 13.93NμB at 7 T and 2 K, whereas for
complex 2, complete saturation was not achieved at 7 T and 2
K [Figure 6 (inset)]. The magnetization value reachs up to
10.07NμB for 2.
The magnetic entropy change ΔSm for complex 1 is
calculated from the magnetization data by using the Maxwell
relation ΔSm(T) = ∫ [∂M(T,H)/∂T]H dH.29,30
the full entropy change per mole of compound corresponding
to two Gd3+
ions is 34.58 J mol−1
, as calculated from the
equation 2R ln(2s + 1), where s = 7/2. So the expected value of
entropy change from complex 1 will be 21.11 J kg−1
calculated value of −ΔSm obtained through magnetization data
is 17.25 J kg−1
at 3 K for ΔH = 7 T (Figure 7). The
observed diﬀerence between the theoretical and experimental
values is due to the antiferromagnetic coupling between the
gadolinium centers in the dimeric unit and high Mw/NGd ratio
of 818.80 (where molecular mass is Mw = 1637.61 g mol−1
NGd = number of gadolinium ions present per mol of the
complex 1), indicating that complex 1 is not a dense magnetic
For complex 2, the plot of M/NμB versus H/T (Figure S12
of the Supporting Information) shows that all isotherm
magnetization curves do not collapse on the same master
curve, indicating the anisotropic nature of the Dy3+
to study the magnetic dynamics of 2, the frequency and
temperature dependencies of the alternating current (ac)
susceptibilities were collected under a zero direct current
(dc) ﬁeld and a 3.5 G ac magnetic ﬁeld (Figure S13 of the
Supporting Information). The out-of-phase frequency-depend-
ent signals below 8 K (Figure 8), indicate the onset of slow
To calculate the anisotropic energy barrier and the relaxation
time, the Debye model and equation: ln(χ″/χ′) = ln(ωτ0) + Ea/
kBT was used.33
The best ﬁtting results give the energy barrier
Ea/kB ≈ 17.73 K and the relaxation time τ0 ≈ 9.7513 × 10−7
(Figure 9), which is consistent with the expected characteristic
relaxation time from 10−6
s for SMMs.34
Cole or Argand plot is shown in Figure S14 of the Supporting
Information, as evidence of the relaxation processes occurring
in complex 2.
Gas Adsorptions Studies. In order to evaluate the porous
property, both complexes were activated under vacuum at 100
°C for 10 h. The PXRD pattern of the activated samples
(Figure S2 of the Supporting Information) of both the
complexes supports the stability of the framework after
activation. The activated samples were introduced with
diﬀerent gases and solvent vapors. Adsorption analyses of 1
and 2 with N2 show almost no uptake at 77 K. The calculated
BET and Langmuir surface areas of complexes 1 and 2 from the
N2 adsorption data were 5 and 11 m2
and 3.2 and 5.3 m2
, respectively. Considerable amount of uptake (8.4 wt % or
) was obtained for CO2 gas at 195 K; this suggests
the selective porous nature of the framework (Figure 10). The
Henry’s Law selectivity for CO2/N2 separation at 273 and 298
K was calculated using the equation Sij = KH(j)/KH(i) (where
KH is Henry’s constant).35
The calculated selectivity of the
framework toward CO2 over N2 is 19 [KH(CO2) = 1.4078 ×
and KH(N2) = 7.2627 × 10−9
Table S3 of the Supporting Information). Such adsorption
Figure 7. ΔSm calculated by using the magnetization data of 1 at
diﬀerent ﬁelds and temperatures.
Figure 8. Temperature dependence of the out-of-phase (χ″) ac
susceptibility for complex 2 at the indicated frequencies and in the
zero dc ﬁeld.
Figure 9. Plot of ln(χ″/χ′) vs reciprocal temperature for 2. Red solid
line represents the ﬁtting in the range of 5.2−8.1 K.
Crystal Growth & Design Article
dx.doi.org/10.1021/cg401804e | Cryst. Growth Des. 2014, 14, 1287−12951291
selectivity of CO2 over N2 may be due to the fact that CO2
molecules have a larger quadrupole moment than N2 and has a
smaller molecular size (CO2, 3.4 Å; N2, 3.1 Å) but bigger
kinetic diameters (CO2, 3.3 Å; N2, 3.6 Å).36
Apart from this, we assume that the 3D framework, which
ions, polar groups, and π-electrons, gives rise to
an electric ﬁeld that interacts with the quadrupole moment of
CO2 to provide extra stabilization energy for adsorption. This is
presumably related to the hydroxyl groups of the pamoate
molecules binding at the open Gd3+
sites and forming H
The sorption characterstics of complex 2 toward
CO2 and N2 shows almost similar behavior as observed for
complex 1 (Figure S15 of the Supporting Information). This
may be due to the analogous framework structure. At 195 K,
the amount of CO2 uptake by the complex 2 is 32.2 cm3
(Figure S15 of the Supporting Information). The slight
diﬀerence in CO2 uptake by complex 2 compared to complex
1 may be due to a slightly less amout of solvent accessible pore
volume. The interaction of CO2 with 1 is also reﬂected in the
value of isosteric heat of adsorption, Qst (23.79 kJ mol−1
low loading of CO2 as calculated by the Dubinin−
Radushkevich (DR) equation40
(Figure 11). For complex 2,
the value of isosteric heat of adsorption, Qst, was found around
14 kJ mol−1
from 298 and 273 K CO2 adsorption isotherm data
(Figure S16 of the Supporting Information).
Vapor Adsorption Studies. Solvent-vapor (H2O, MeOH,
and CH3CN at 298 K) adsorption studies further conﬁrms the
selective polar porosity of the complexes. The activated
powdered samples of both the complexes were exposed to
diﬀerent solvent vapors in closed vessels for 24 h. PXRD
patterns of the vapor-exposed samples indicate the retention of
the framework stability for both complexes (Figure S2 of the
Supporting Information). The MeOH adsorption proﬁle shows
less uptake in the low-pressure region and then gradually
increased up to a 0.9 P/Po pressure, and a steep rise occurred in
the isotherm. The ﬁnal uptake from the proﬁle was found to be
for complex 1. The lower adsorption amounts of
complex 1 with other solvent vapors (CH3CN and H2O)
further justiﬁes the high polar nature of the pore surfaces
(Figure 12). Although H2O is more polar than MeOH, the
lower adsorption amount might be due to the coordination of
adsorbed water molecules to the Gd3+
center and the hydrogen-
bonding interactions between the framework and adsorbed
The PXRD pattern of the water-adsorbed
sample in comparison with the as-synthesized one is further
supported that water-loaded complex 1 possesses a similar
structure to the as-synthesized one (Figure S2 of the
Supporting Information). Due to the high polarity of methanol,
it can interact eﬀectively with the framework through diﬀerent
hydrogen-bonding (O−H···O/N) interactions between free
−OH from pamoate and coordinated oxygen and nitrogen
atoms from DMF.41,42
This type of selectivity toward MeOH
over other solvents has important implications in the separation
of the mixture of solvents. Separation of MeOH over H2O
might be of more practical importance and can be employed to
generate high purity MeOH. The selectivity of the framework
toward MeOH vapor over CH3CN and H2O might be due to
the well ﬁt of MeOH molecules inside the pore, which causes
stronger interactions with the MOF.41c
Similar solvent vapor
adsorption studies were also carried out for complex 2. The
results illustrate that complex 2 also shows selectivity toward
methanol vapor (Figure S17). The lower uptake of methanol
) for complex 2 compared to complex 1 may be
due to a lower amout of solvent accessible pore volume
Figure 10. CO2 and N2 adsorption isotherm observed for complex 1,
at diﬀerent temperatures (blue, 195 K; black, 273 K; and red, 298 K
for CO2 and magenta 273 K, yellow 298 K for N2) (closed and open
symbols represent adsorption and desorption branches, respectively).
Figure 11. CO2 isosteric heat of adsorption using adsorption data for
complex 1 collected at 273 and 298 K.
Figure 12. Solvent vapor adsorption isotherm observed for complex 1;
MeOH, (blue) H2O (black), and CH3CN (red) at 298 K.
Crystal Growth & Design Article
dx.doi.org/10.1021/cg401804e | Cryst. Growth Des. 2014, 14, 1287−12951292
available in complex 2 compared to that of 1 (6226.5 Å3
complex 1 and 5766.2 Å3
for complex 2).
Photophysical Properties. The π-conjugated organic
ligands, which usually have strongly absorbing chromophoric
properties, were used eﬀectively as sensitive reagents for
tailoring lanthanide luminescence.43
Although pamoate exhibits
extended π-conjugated naphthalene moieties, the solid state
photophysical properties of its lanthanide complexes are not
known so far. The photoluminescence spectra of the pamoic
acid and complexes 1 and 2 were measured in the solid state at
room temperature (Figure 13). On excitation at 430 nm
(Figure S18 of the Supporting Information), complexes 1 and 2
exhibit a sharp emission peak at ∼467 nm and a broad peak at
∼555 nm, respectively. To get an insight into the nature of
emission of complexes 1 and 2, the emission spectra of ligand
“pamoic acid” was measured. The sharp emission peak at
around ∼464 nm (λex = 430 nm) was observed. The sharp
emission peak at ∼467 nm for 1 and 2 were similar to that of
the ligand, indicating that they were attributed to the emission
from the ligand. For complex 2 (Dy3+
), the broad emission
peak observed in the region of 470−670 nm might be due to
the overlap of two peaks originating from the transition 4
H15/2 and 4
H13/2, which corresponds to the character-
istic blue emission of the Dy3+
luminescence intensity of complexes 1 and 2 are similar in
the 470−670 nm region, which might be due to the similar
framework arrangements. So, the aforementioned photo-
luminescent behavior of both complexes demonstrates that
they may be potential candidates for photoluminescent
We have reported synthesis and characterization of two
isostructural 3D lanthanide-based MOFs. We choose lantha-
nides as metal centers as an attempt to explore the metal-
centric properties (e.g., photoluminescent and magnetic) of
MOFs, in addition to the properties related to pore size and
surface area. The magnetic characterization reveals that
complex 1 shows cryogenic magnetic refrigeration property,
whereas 2 shows slow magnetic relaxation. Complexes 1 and 2
exhibit high methanol vapor uptake and shows selectivity in
sorption toward CO2 over N2. From the structural revelation
and ﬂuoresence property study, it can be concluded that the
ligand pamoic acid provides a good metal-to-metal distance for
large pore size and also behaves like a suitable chromophoric
moiety (antena) for sensitization of the lanthanides. Further
work with other lanthanides are under way.
■ ASSOCIATED CONTENT
*S Supporting Information
Additional data and plots on spectroscopic characterizations,
magnetic, PXRD, and gas sorption studies.This material is
available free of charge via the Internet at http://pubs.acs.org.
CCDC 941734 and 942172 contains supplementary crystallo-
graphic data for this paper.
■ AUTHOR INFORMATION
*E-mail: firstname.lastname@example.org. Fax: +91-755-6692392. Tel: +91-
The authors declare no competing ﬁnancial interest.
S.B., S.G., and S.S. thank IISER Bhopal for the Ph.D.
fellowships. H.S.J. thanks IISER Bhopal for the post-doctoral
fellowship. S.K. thanks DST (Project No. SR/FT/CS-016/
2010), CSIR (Project No. 01(2473)/11/EMR II), the
government of India, and IISER Bhopal for generous ﬁnancial
and infrastructural support.
(1) (a) Farha, O. K.; Eryazici, I.; Jeong, N. C.; Hauser, B. G.; Wilmer,
C. E.; Sarjeant, A. A.; Snurr, R. Q.; Nguyen, S. T.; Yazaydın, A. O.;
Hupp, J. T. J. Am. Chem. Soc. 2012, 134, 15016−15021. (b) Koh, K.;
Wong-Foy, A. G.; Matzger, A. J. J. Am. Chem. Soc. 2009, 131, 4184−
4185. (c) Furukawa, H.; Ko, N.; Go, Y. B.; Aratani, N.; Choi, S. B.;
Choi, E.; Yazaydın, A. Ö.; Snurr, R. Q.; O’Keeffe, M.; Kim, J.; Yaghi,
O. M. Science 2010, 329, 424−428. (d) Farha, O. K.; Yazaydın, A. O.;
Eryazici, I.; Malliakas, C. D.; Hauser, B. G.; Kanatzidis, M. G.; Nguyen,
S. T.; Snurr, R. Q.; Hupp, J. T. Nat. Chem. 2010, 2, 944−948.
(2) (a) Uemura, T.; Yanaia, N.; Kitagawa, S. Chem. Soc. Rev. 2009, 38,
1228−1236. (b) Kitagawa, S.; Kitaura, R.; Noro, S. Angew. Chem., Int.
Ed. 2004, 43, 2334−2375. (c) Yaghi, O. M.; O’Keeffe, M.; Ockwig, N.
W.; Chae, H. K.; Eddaoudi, M.; Kim, J. Nature 2003, 423, 705−714.
(d) Kepert, C. J. Chem. Commun. 2006, 695−700.
(3) (a) Tranchemontagne, D. J.; Mendoza-Cortes, J. L.; O’Keeffe,
M.; Yaghi, O. M. Chem. Soc. Rev. 2009, 38, 1257−1283. (b) Hurd, J.
A.; Vaidhyanathan, R.; Thangadurai, V.; Ratcliffe, C. I.; Moudrakovski,
I. L.; Shimizu, G. K. H. Nat. Chem. 2009, 1, 705−710. (c) Farha, O. K.;
Hupp, J. T. Acc. Chem. Res. 2010, 43, 1166−1175. (d) Horcajada, P.;
Serre, C.; Vallet-Regí, M.; Sebban, M.; Taulelle, F.; Ferey, G. Angew.
Chem., Int. Ed. 2006, 45, 5974−5978. (e) Rocca, J. D.; Liu, D.; Lin, W.
Acc. Chem. Res. 2011, 44, 957−968.
(4) (a) Sakata, Y.; Furukawa, S.; Kondo, M.; Hirai, K.; Horike, N.;
Takashima, Y.; Uehara, H.; Louvain, N.; Meilikhov, M.; Tsuruoka, T.;
Isoda, S.; Kosaka, W.; Sakata, O.; Kitagawa, S. Science 2013, 339, 193−
196. (b) Shimomura, S.; Higuchi, M.; Matsuda, R.; Yoneda, K.;
Hijikata, Y.; Kubota, Y.; Mita, Y.; Kim, J.; Takata, M.; Kitagawa, S. Nat.
Chem. 2010, 2, 633−637. (c) Yanai, N.; Kitayama, K.; Hijikata, Y.;
Sato, H.; Matsuda, R.; Kubota, Y.; Takata, M.; Mizuno, M.; Uemura,
T.; Kitagawa, S. Nat. Mater. 2011, 10, 787−793. (d) Uemura, K.;
Kitagawa, S. Chem. Soc. Rev. 2005, 34, 109−119.
(5) (a) Li, H.; Eddaoudi, M.; O’Keeffe, M.; Yaghi, O. M. Nature
1999, 402, 276−279. (b) Ockwig, N.; Friedrichs, O.; O’Keefee, M.;
Yaghi, O. M. Acc. Chem. Res. 2005, 38, 176−182. (c) Wang, B.; Cote,
Figure 13. Solid state emission spectra of ligand pamoic acid and
complexes 1 and 2 at room temperature.
Crystal Growth & Design Article
dx.doi.org/10.1021/cg401804e | Cryst. Growth Des. 2014, 14, 1287−12951293
A. P.; Furukawa, H.; O’Keeffe, M.; Yaghi, O. M. Nature 2008, 453,
207−211. (d) Deng, H.; Grunder, S.; Cordova, K. E.; Valente, C.;
Furukawa, H.; Hmadeh, M.; Gandara, F.; Whalley, A. C.; Liu, Z.;
Asahina, S.; Kazumori, H.; O’Keeffe, M.; Terasaki, O.; Stoddart, J. F.;
Yaghi, O. M. Science 2012, 336, 1018−1023.
(6) (a) Ferey, G. Chem. Soc. Rev. 2008, 37, 191−214. (b) Mellot-
Draznieks, C.; Serre, C.; Millange, F.; Dutour, J.; Surble, S.; Margiolaki,
I.; Ferey, G. Science 2005, 309, 2040−2042. (c) Latroche, M.; Surble,
S.; Serre, C.; Mellot-Draznieks, C.; Llewellyn, P. L.; Lee, J. H.; Chang,
J. S.; Jhung, S. H.; Ferey, G. Angew. Chem., Int. Ed. 2006, 45, 8227−
(7) Jeong, N. C.; Samanta, B.; Lee, C. Y.; Farha, O. K.; Hupp, J. T. J.
Am. Chem. Soc. 2012, 134, 51−54.
(8) (a) Hasell, T.; Wu, X.; Jones, J. T. A.; Bacsa, J.; Steiner, A.; Mitra,
T.; Trewin, A.; Adams, D. J.; Cooper, A. I. Nat. Chem. 2010, 2, 750−
755. (b) Holst, J. R.; Trewin, A.; Cooper, A. I. Nat. Chem. 2010, 2,
(9) (a) Zhao, X.; Xiao, B.; Fletcher, A. J.; Thomas, K. M.; Bradshaw,
D.; Rosseinsky, M. J. Science 2004, 306, 1012−1015. (b) Swamy, S. I.;
Bacsa, J.; Jones, J. T. A.; Stylianou, K. C.; Steiner, A.; Ritchie, L. K.;
Hasell, T.; Gould, J. A.; Laybourn, A.; Khimyak, Y. Z.; Adams, D. J.;
Rosseinsky, M. J.; Cooper, A. I. J. Am. Chem. Soc. 2010, 132, 12773−
(10) (a) Park, J.; Yuan, D.; Pham, K. T.; Li, J. R.; Yakovenko, A.;
Zhou, H. C. J. Am. Chem. Soc. 2012, 134, 99−102. (b) Li, J. R.; Zhou,
H. C. Nat. Chem. 2010, 2, 893−898.
(11) (a) Gagnon, K. J.; Beavers, C. M.; Clearfield, A. J. Am. Chem.
Soc. 2013, 135, 1252−1255. (b) Poojary, D. M.; Zhang, B.; Clearfield,
A. J. Am. Chem. Soc. 1997, 119, 12550−12559. (c) Gagnon, K. J.;
Perry, H. P.; Clearfield, A. Chem. Rev. 2012, 112, 1034−1054.
(12) (a) Chapman, K. W.; Halder, G. J.; Chupas, P. J. J. Am. Chem.
Soc. 2008, 130, 10524−10526. (b) Chapman, K. W.; Halder, G. J.;
Chupas, P. J. J. Am. Chem. Soc. 2009, 131, 17546−17547. (c) Sava, D.
F.; Rodriguez, M. A.; Chapman, K. W.; Chupas, P. J.; Greathouse, J.
A.; Crozier, P. S.; Nenoff, T. M. J. Am. Chem. Soc. 2011, 133, 12398−
(13) (a) Li, W.; Probert, M. R.; Kosa, M.; Bennett, T. D.;
Thirumurugan, A.; Burwood, R. P.; Parinello, M.; Howard, J. A. K.;
Cheetham, A. K. J. Am. Chem. Soc. 2012, 134, 11940−11943. (b) Tan,
J. C.; Cheetham, A. K. Chem. Soc. Rev. 2011, 40, 1059−1080.
(c) Horcajada, P.; Gref, R.; Baati, T.; Allan, P. K.; Maurin, G.;
Couvreur, P.; Ferey, G.; Morris, R. E.; Serre, C. Chem. Rev. 2012, 112,
1232−1268. (d) Chalati, T.; Horcajada, P.; Gref, R.; Couvreura, P.;
Serre, C. J. Mater. Chem. 2011, 21, 2220−2227. (e) Vaidhyanathan, R.;
Natarajan, S.; Rao, C. N. R. Dalton Trans. 2003, 1459−1464.
(f) Vaidhyanathan, R.; Natarajan, S.; Rao, C. N. R. Cryst. Growth
Des. 2003, 3, 47−51.
(14) (a) Benelli, C.; Gatteschi, D. Chem. Rev. 2002, 102, 2369−2388.
(b) Han, Y. F.; Li, X. Y.; Li, L. Q.; Ma, C. L.; Shen, Z.; Song, Y.; You,
X. Z. Inorg. Chem. 2010, 49, 10781−10787. (c) Coronado, E.;
Espallargas, M. Chem. Soc. Rev. 2013, 42, 1525−1539. (d) Dechambe-
noit, P.; Long, J. R. Chem. Soc. Rev. 2011, 40, 3249−3265.
(e) Maspoch, D.; Ruiz-Molinaa, D.; Veciana, J. Chem. Soc. Rev.
2007, 36, 770−818.
(15) (a) Binnemans, K. Chem. Rev. 2009, 109, 4283−4374.
(b) Rocha, J.; Carlos, L. D.; Paz, F. A. A.; Ananiasa, D. Chem. Soc.
Rev. 2011, 40, 926−940. (c) Allendorf, M. D.; Bauer, C. A.; Bhakta, R.
K.; Houka, R. J. T. Chem. Soc. Rev. 2009, 38, 1330−1352. (d) Carlos,
L. D.; Ferreira, R. A. S.; Bermudez, V.; Lopez, B. J.; Escribano, P.
Chem. Soc. Rev. 2011, 40, 536−549. (e) Li, Z. Y.; Zhu, G. S.; Guo, X.
D.; Zhao, X. J.; Jin, Z.; Qiu, S. L. Inorg. Chem. 2007, 46, 5174−5178.
(16) (a) Jia, J. H.; Lin, X.; Blake, A. J.; Champness, N. R.;
Hubberstey, P.; Shao, L. M.; Walker, G.; Wilson, C.; Schröder, M.
Inorg. Chem. 2006, 45, 8838−8840. (b) Chandler, B. D.; Yu, J. O.;
Cramb, D. T.; Shimizu, G. K. H. Chem. Mater. 2007, 19, 4467−4473.
(17) (a) Zhao, B.; Cheng, P.; Dai, Y.; Cheng, C.; Liao, D. Z.; Yan, S.
P.; Jiang, Z. H.; Wang, G. L. Angew Chem. Int. Ed. 2003, 42, 934−936.
(b) Zhao, B.; Cheng, P.; Chen, X. Y.; Cheng, C.; Shi, W.; Liao, D. Z.;
Yan, S. P.; Jiang, Z. H. J. Am. Chem. Soc. 2004, 126, 3012−3013.
(c) Zhao, B.; Chen, X. Y.; Cheng, P.; Liao, D. Z.; Yan, S. P.; Jiang, Z.
H. J. Am. Chem. Soc. 2004, 126, 15394−15395. (e) Zhao, X. Q.; Zhao,
B.; Ma, Y.; Shi, W.; Cheng, P.; Jiang, Z. H.; Liao, D. Z.; Yan, S. P. Inorg.
Chem. 2007, 46, 5832−5834. (f) Chen, Z.; Zhao, B.; Cheng, P.; Zhao,
X. Q.; Shi, W.; Song, Y. Inorg. Chem. 2009, 48, 3493−3495.
(18) (a) Du, M.; Li, C.-P.; Zhao, X.-J.; Yu, Q. CrystEngComm 2007,
9, 1011−1028. (b) Wang, S.; Yun, R.; Peng, Y.; Zhang, Q.; Lu, J.; Dou,
J.; Bai, J.; Li, D.; Wang, D. Cryst. Growth Des. 2012, 12, 79−92.
(c) Wang, S.; Peng, Y.; Wei, X.; Zhang, Q.; Wang, D.; Dou, J.; Lia, D.;
Bai, J. CrystEngComm 2011, 13, 5313−5316. (d) Shi, X.-M.; Li, M.-X.;
He, X.; Liu, H.-J.; Shao, M. Polyhedron 2010, 29, 2075−2080.
(e) Wang, J.-J.; Yang, M.-L.; Hu, H.-M.; Xue, G.-L.; Li, D.-S.; Shi, Q.-
Z. Inorg. Chem. Commun. 2007, 10, 269−272. (f) Shi, Q.; Sun, Y.;
Sheng, L.; Ma, K.; Hu, M.; Hu, X.; Huang, S. Cryst. Growth Des. 2008,
8, 3401−3407. (g) Han, Z.-X.; Wanga, J.-J.; Hua, H.-M.; Chen, X.-L.;
Wua, Q.-R.; Li, D.-S.; Shi, Q.-Z. J. Mol. Struct. 2008, 891, 364−369.
(h) Li, N.; Gou, L.; Hua, H.-M.; Chen, S.-H.; Chen, X.-L.; Wang, B.-
C.; Wua, Q.-R.; Yang, M.-L.; Xue, G.-L. Inorg. Chim. Acta 2009, 362,
3475−3483. (i) Baghel, G. S.; Rao, C. P. Polyhedron 2009, 28, 3507−
(19) Kahn, O. Molecular Magnetism; Wiley-VCH: New York, 1991.
(20) Sheldrick, G. M. SHELXTL: Program for the Solution of Crystal of
Structures; University of Göttingen: Göttingen, Germany, 1993.
(21) Sheldrick, G. M. SHELXL 97: Program for Crystal Structure
Reﬁnement; University of Göttingen: Göttingen, Germany, 1997.
(22) Spek, A. L. J. Appl. Crystallogr. 2003, 36, 7−13.
(23) Farrugia, L. J. J. Appl. Crystallogr. 1999, 32, 837−838.
(24) (a) Munakata, M.; Wu, L. P.; Kuroda-Sowa, T.; Maekawa, M.;
Suenaga, Y.; Sugimoto, K. Inorg. Chem. 1997, 36, 4903−4905.
(b) Munakata, M.; Wu, L. P.; Ning, G. L.; Kuroda-Sowa, T.;
Maekawa, M.; Suenaga, Y.; Maeno, N. J. Am. Chem. Soc. 1999, 121,
4968−4976. (c) Grummt, U. W.; Birckner, E.; Klemm, E.; Egbe, D. A.
M.; Heise, B. J. Phys. Org. Chem. 2000, 13, 112−126. (d) Fu, R.; Xiang,
S.; Hu, S.; Wang, L.; Li, Y.; Huang, X.; Wu, X. Chem. Commun. 2005,
(25) Deacon, G. B.; Phillips, R. J. Coord. Chem. Rev. 1980, 33, 227−
(26) Spek, A. L. PLATON: A Multipurpose Crystallographic Tool;
Utrecht University: Utrecht, The Netherlands, 2001.
(27) (a) Koberl, M.; Cokoja, M.; Herrmann, W. A.; Kuhn, F. E.
Dalton Trans. 2011, 40, 6834−6859. (b) Yu, L. Q.; Huang, R. D.; Xu,
Y. Q.; Liu, T. F.; Chu, W.; Hu, C. W. Inorg. Chim. Acta 2008, 361,
2115−2122. (c) Su, S.; Chen, W.; Qin, W.; Qin, C.; Song, S.; Guo, Z.;
Li, G.; Song, S.; Zhu, M.; Wang, S.; Hao, S.; Zhang, H. Cryst. Growth
Des. 2012, 12, 1808−1815. (d) Zhu, X.; Lu, J.; Li, X.; Gao, S.; Li, G.;
Xiao, F.; Cao, R. Cryst. Growth Des. 2008, 8, 1897−1901.
(28) (a) John, D.; Urland, W. Eur. J. Inorg. Chem. 2006, 3503−3509.
(b) Rodhe, A.; Urland, W. Dalton Trans. 2006, 2974−2978.
(c) Delgado, L. C.; Fabelo, O.; Cano, J.; Pasan, J.; Delgado, F. S.;
Lloret, F.; Julve, M.; Perez, C. R. CrystEngComm 2009, 11, 2131−
2142. (d) Sun, Y. G.; Jiang, B.; Cui, T. F.; Xiong, G.; Smet, P. F.; Ding,
F.; Gao, E. N.; Lv, T.; Eeckhout, K. V.; Poelman, D.; Verpoort, F.
Dalton Trans. 2011, 40, 11581−11590. (e) Majeed, J.; Mondal, K. C.;
Kostakis, G. E.; Lan, Y.; Anson, C. E.; Powell, A. K. Chem. Commun.
2010, 46, 2551−2553.
(29) (a) Colacio, E.; Ruiz, G.; Lorusso, G.; Brechin, E. K.; Evangelisti,
M. Chem. Commun. 2013, 49, 3845−3847. (b) Zheng, Y. Z.;
Evangelisti, M.; Winpenny, R. E. P. Angew. Chem., Int. Ed. 2011, 50,
3692−3695. (c) Langley, S. K.; Chilton, N. F.; Moubaraki, B.; Hooper,
T.; Brechin, E. K.; Evangelisti, M.; Murray, K. S. Chem. Sci. 2011, 2,
1166−1169. (d) Guo, F. S.; Chen, Y. C.; Liu, J.-L.; Leng, J.-D.; Meng,
Z. S.; Vrábel, P.; Orendáč, M.; Tong, M.-L. Chem. Commun. 2012, 48,
12219−12221. (e) Guo, F.-S.; Leng, J. D.; Liu, J. L.; Meng, Z. S.;
Tong, M. L. Inorg. Chem. 2012, 51, 405−413. (f) Goswami, S.;
Adhikary, A.; Jena, H. S.; Konar, S. Dalton Trans. 2013, 42, 9813−
9817. (g) Biswas, S.; Adhikary, A.; Goswami, S.; Konar, S. Dalton
Trans. 2013, 42, 13331−13334. (h) Chang, L. X; Xiong, G.; Wang, L.;
Cheng, P.; Zhao, B. Chem. Commun. 2013, 49, 1055−1057. (i) Shi, P.
Crystal Growth & Design Article
dx.doi.org/10.1021/cg401804e | Cryst. Growth Des. 2014, 14, 1287−12951294
F.; Zheng, Y. Z.; Zhao, X. Q; Xiong, G.; Zhao, B.; Wan, F. F; Cheng, P.
Chem.Eur. J. 2012, 18, 15086−15091.
(30) (a) Hooper, T. N.; Schnack, J.; Piligkos, S.; Evangelisti, M.;
Brechin, E. K. Angew. Chem., Int. Ed. 2012, 51, 4633−4636.
(b) Evangelisti, M.; Brechin, E. K. Dalton Trans. 2010, 39, 4672−
4676. (c) Evangelisti, M.; Luis, F.; de Jongh, L. J.; Affronte, M. J.
Mater. Chem. 2006, 16, 2534−2549. (d) Sibille, R.; Mazet, T.;
Malaman, B.; François, M. Chem.−Eur. J. 2012, 18, 12970−12973.
(e) Zheng, Y. Z.; Evangelisti, M.; Tuna, F.; Winpenny, R. E. P. J. Am.
Chem. Soc. 2012, 134, 1057−1065. (f) Karotsis, G.; Evangelisti, M.;
Dalgarno, S. J.; Brechin, E. K. Angew. Chem., Int. Ed. 2009, 48, 9928−
9931. (g) Hou, Y. L.; Xiong, G.; Shi, P. F.; Cheng, R. R.; Zhong, J. C.;
Zhao, B. Chem. Commun. 2013, 49, 6066−6068. (h) Wu, M.; Jiang, F.;
Kong, X.; Yuan, D.; Long, L.; AL-Thabaiti, S. A.; Hong, M. Chem. Sci.
2013, 4, 3104−3109.
(31) (a) Zhao, L.; Xue, S.; Tang, J. Inorg. Chem. 2012, 51, 5994−
5996. (b) Gass, I. A.; Moubaraki, B.; Langley, S. K.; Batten, S. R.;
Murray, K. S. Chem. Commun. 2012, 48, 2089−2091.
(32) (a) Hou, Y. L.; Xiong, G.; Shen, B.; Zhao, B.; Chen, Z.; Cui, J. Z.
Dalton Trans. 2013, 42, 3587−3596. (b) Habib, F.; Lin, P. H.; Long, J.;
Korobkov, I.; Wernsdorfer, W.; Murugesu, M. J. Am. Chem. Soc. 2011,
133, 8830−8833. (c) Gamer, M. T.; Lan, Y.; Roesky, P. W.; Powell, A.
K.; Clerac, R. Inorg. Chem. 2008, 47, 6581−6583. (d) Ke, H. S.; Xu, G.
F.; Zhao, L.; Tang, J. K.; Zhang, X. Y.; Zhang, H. J. Chem.Eur. J.
2009, 15, 10335−10338.
(33) (a) Bartolomé, J.; Filoti, G.; Kuncser, V.; Schinteie, G.;
Mereacre, V.; Anson, C. E.; Powell, A. K.; Prodius, D.; Turta, C. Phys.
Rev. B 2009, 80, 014430−014446. (b) Lin, S. Y.; Xu, G. F.; Zhao, L.;
Guo, Y. N.; Guo, Y.; Tang, J. K. Dalton Trans. 2011, 40, 8213−8217.
(34) (a) Lin, S.-Y.; Zhao, L.; Ke, H.; Guo, Y.-N.; Tang, J.; Guo, Y.;
Dou, J. Dalton Trans. 2012, 41, 3248−3252. (b) Mishra, A.;
Wernsdorfer, W.; Abboud, A. K.; Christou, G. J. Am. Chem. Soc.
2004, 126, 15648−15649.
(35) (a) Nagarkar, S. S.; Chaudhari, A. K.; Ghosh, S. K. Inorg. Chem.
2012, 51, 572−576. (b) Chen, Z.; Xiang, S.; Arman, H. D.; Mondal, J.
U.; Li, P.; Zhao, D.; Chen, B. Inorg. Chem. 2011, 50, 3442−3446.
(36) (a) Liu, J.; Thallapally, P. K.; McGrail, B. P.; Brown, D. R.; Liu,
J. Chem. Soc. Rev. 2012, 41, 2308−2322. (b) Cui, P.; Ma, Y. G.; Li, H.
H.; Zhao, B.; Li, J. R.; Cheng, P.; Balbuena, P. B.; Zhou, H. C. J. Am.
Chem. Soc. 2012, 134, 18892−18895. (c) Li, J. R.; Yu, J.; Lu, W.; Sun,
L. B.; Balbuena, P. B.; Zhou, H. C. Nat. Commun. 2013,
DOI: 10.1038/ncomms2552. (d) Li, J. R.; Ma, Y.; McCarthy, M. C.;
Sculley, J.; Yu, J.; Jeong, H. K.; Balbuena, P. B.; Zhou, H. C. Coord.
Chem. Rev. 2011, 255, 1791−1823.
(37) (a) Kong, X.; Scott, E.; Ding, W.; Mason, J. A.; Long, J. R.;
Reimer, J. A. J. Am. Chem. Soc. 2012, 134, 14341−14344. (b) Lin, L.
C.; Kim, J.; Kong, X.; Scott, E.; McDonald, T. M.; Long, J. R.; Reimer,
J. A.; Smit, B. Angew. Chem., Int. Ed. 2013, 52, 4410−4413.
(c) Jayaramulu, K.; Reddy, S. K.; Hazra, A.; Balasubramanian, S.;
Maji, T. K. Inorg. Chem. 2012, 51, 7103−7111. (d) Li, J. R.; Kuppler,
R. J.; Zhou, H. C. Chem. Soc. Rev. 2009, 38, 1477−1504. (e) Kanoo, P.;
Mostafa, G.; Matsuda, R.; Kitagawa, S.; Maji, T. K. Chem. Commun.
2011, 47, 8106−8108.
(38) (a) Sumida, K.; Rogow, D. L.; Mason, J. A.; McDonald, T. M.;
Bloch, E. D.; Herm, Z. R.; Bae, T. H.; Long, J. R. Chem. Rev. 2012,
112, 724−781. (b) Park, H. J.; Suh, M. P. Chem. Sci. 2013, 4, 685−690.
(c) Choi, H. S.; Suh, M. P. Angew. Chem., Int. Ed. 2009, 48, 6865−
6869. (d) Kim, T. K.; Suh, M. P. Chem. Commun. 2011, 47, 4258−
(39) (a) Bae, Y. S.; Farha, O. K.; Hupp, J. T.; Snurr, R. Q. J. Mater.
Chem. 2009, 19, 2131−2134. (b) Wilmer, C. E.; Farha, O. K.; Bae, Y.
S.; Hupp, J. T.; Snurr, R. Q. Energy Environ. Sci. 2012, 5, 9849−9856.
(c) Kuppler, R. J.; Timmons, D. J.; Fang, Q.-R.; Li, J.-R.; Makal, T. A.;
Young, M. D.; Yuan, D.; Zhao, D.; Zhuang, W.; Zhou, H.-C. Coord.
Chem. Rev. 2009, 253, 3042−3066.
(40) Dubinin, M. M. Chem. Rev. 1960, 60, 235−241.
(41) (a) Kanoo, P.; Sambhu, R.; Maji, T. K. Inorg. Chem. 2011, 50,
400−402. (b) Li, H.; Shi, W.; Zhao, K.; Niu, Z.; Chen, X.; Cheng, P.
Chem.Eur. J. 2012, 18, 5715−5723. (c) Huang, Q.; Cai, J.; Wu, H.;
He, Y.; Chen, B.; Qian, G. J. Mater. Chem. 2012, 22, 10352−10355.
(d) Lin, Z.; Zou, R.; Liang, J.; Xia, W.; Xia, D.; Wang, Y.; Wang, Y.;
Lin, J.; Hu, T.; Chen, Q.; Wang, X.; Zhao, Y.; Burrel, A. K. J. Mater.
Chem. 2012, 22, 7813−7818. (e) Han, L.; Yan, Y.; Sun, F.; Cai, K.;
Borjigin, T.; Zhao, X.; Qu, F.; Zhu, G. Cryst. Growth Des. 2013, 13,
(42) (a) Maji, T. K.; Uemura, K.; Chang, H. C.; Matsuda, R.;
Kitagawa, S. Angew. Chem., Int. Ed. 2004, 43, 3269−3272. (b) Ghosh,
S. K.; Bureekaew, S.; Kitagawa, S. Angew. Chem., Int. Ed. 2008, 47,
3403−3406. (c) Sadakiyo, M.; Yamada, T.; Kitagawa, H. J. Am. Chem.
Soc. 2011, 133, 11050−11053. (d) Wu, H.; Gong, Q.; Olson, D. H.; Li,
J. Chem. Rev. 2012, 112, 836−868.
(43) (a) Yersin, H.; Vogler, A. Photochemistry and Photophysics of
Coordination Compounds; Springer-Verlag: Berlin, 1987. (b) Xu, J. G.;
Wang, Z. B. Fluorescence Analytical Methods; Chinese Science
Publishing Company: Beijing, 2006.
(44) (a) Liu, S.-J.; Huang, Y.; Lin, Z.-J.; Lib, X.-F.; Cao, R. RSC Adv.
2013, 3, 9279−9287. (d) Jung, S. H.; Yoon, S. K.; Kim, J. S. G.; Kang,
J. G. Bull. Korean Chem. Soc. 1992, 13, 650−654.
Crystal Growth & Design Article
dx.doi.org/10.1021/cg401804e | Cryst. Growth Des. 2014, 14, 1287−12951295